1 Overview of Rapid Prototyping
The term rapid prototyping (RP) refers to a class of technologies that can automatically construct
physical models from Computer-Aided Design (CAD) data. These "three dimensional printers"
allow designers to quickly create tangible prototypes of their designs, rather than just two-
dimensional pictures. Such models have numerous uses. They make excellent visual aids for
communicating ideas with co-workers or customers. In addition, prototypes can be used for
design testing. For example, an aerospace engineer might mount a model airfoil in a wind tunnel
to measure lift and drag forces. Designers have always utilized prototypes; RP allows them to be
made faster and less expensively.
In addition to prototypes, RP techniques can also be used to make tooling (referred to as rapid
tooling) and even production-quality parts (rapid manufacturing). For small production runs and
complicated objects, rapid prototyping is often the best manufacturing process available. Of
course, "rapid" is a relative term. Most prototypes require from three to seventy-two hours to
build, depending on the size and complexity of the object. This may seem slow, but it is much
faster than the weeks or months required to make a prototype by traditional means such as
machining. These dramatic time savings allow manufacturers to bring products to market faster
and more cheaply. In 1994, Pratt & Whitney achieved "an order of magnitude [cost] reduction
[and] . . . time savings of 70 to 90 percent" by incorporating rapid prototyping into their
investment casting process. 5
At least six different rapid prototyping techniques are commercially available, each with unique
strengths. Because RP technologies are being increasingly used in non-prototyping applications,
the techniques are often collectively referred to as solid free-form fabrication, computer
automated manufacturing, or layered manufacturing. The latter term is particularly descriptive
of the manufacturing process used by all commercial techniques. A software package "slices" the
CAD model into a number of thin (~0.1 mm) layers, which are then built up one atop another.
Rapid prototyping is an "additive" process, combining layers of paper, wax, or plastic to create a
solid object. In contrast, most machining processes (milling, drilling, grinding, etc.) are
"subtractive" processes that remove material from a solid block. RP’s additive nature allows it to
create objects with complicated internal features that cannot be manufactured by other means.
Of course, rapid prototyping is not perfect. Part volume is generally limited to 0.125 cubic
meters or less, depending on the RP machine. Metal prototypes are difficult to make, though this
should change in the near future. For metal parts, large production runs, or simple objects,
conventional manufacturing techniques are usually more economical. These limitations aside,
rapid prototyping is a remarkable technology that is revolutionizing the manufacturing process.
2 The Basic Process
2. Although several rapid prototyping techniques exist, all employ the same basic five-step process.
The steps are:
1. Create a CAD model of the design
2. Convert the CAD model to STL format
3. Slice the STL file into thin cross-sectional layers
4. Construct the model one layer atop another
5. Clean and finish the model
CAD Model Creation: First, the object to be built is modeled using a Computer-Aided Design
(CAD) software package. Solid modelers, such as Pro/ENGINEER, tend to represent 3-D objects
more accurately than wire-frame modelers such as AutoCAD, and will therefore yield better
results. The designer can use a pre-existing CAD file or may wish to create one expressly for
prototyping purposes. This process is identical for all of the RP build techniques.
Conversion to STL Format: The various CAD packages use a number of different algorithms
to represent solid objects. To establish consistency, the STL (stereolithography, the first RP
technique) format has been adopted as the standard of the rapid prototyping industry. The second
step, therefore, is to convert the CAD file into STL format. This format represents a three-
dimensional surface as an assembly of planar triangles, "like the facets of a cut jewel." 6
contains the coordinates of the vertices and the direction of the outward normal of each triangle.
Because STL files use planar elements, they cannot represent curved surfaces exactly. Increasing
the number of triangles improves the approximation, but at the cost of bigger file size. Large,
complicated files require more time to pre-process and build, so the designer must balance
accuracy with manageablility to produce a useful STL file. Since the .stl format is universal, this
process is identical for all of the RP build techniques.
Slice the STL File: In the third step, a pre-processing program prepares the STL file to be built.
Several programs are available, and most allow the user to adjust the size, location and
orientation of the model. Build orientation is important for several reasons. First, properties of
rapid prototypes vary from one coordinate direction to another. For example, prototypes are
usually weaker and less accurate in the z (vertical) direction than in the x-y plane. In addition,
part orientation partially determines the amount of time required to build the model. Placing the
shortest dimension in the z direction reduces the number of layers, thereby shortening build time.
The pre-processing software slices the STL model into a number of layers from 0.01 mm to 0.7
mm thick, depending on the build technique. The program may also generate an auxiliary
structure to support the model during the build. Supports are useful for delicate features such as
overhangs, internal cavities, and thin-walled sections. Each PR machine manufacturer supplies
their own proprietary pre-processing software.
Layer by Layer Construction: The fourth step is the actual construction of the part. Using one
of several techniques (described in the next section) RP machines build one layer at a time from
polymers, paper, or powdered metal. Most machines are fairly autonomous, needing little human
3. Clean and Finish: The final step is post-processing. This involves removing the prototype from
the machine and detaching any supports. Some photosensitive materials need to be fully cured
before use. Prototypes may also require minor cleaning and surface treatment. Sanding, sealing,
and/or painting the model will improve its appearance and durability.
3 Rapid Prototyping Techniques
Most commercially available rapid prototyping machines use one of six techniques. At present,
trade restrictions severely limit the import/export of rapid prototyping machines, so this guide
only covers systems available in the U.S.
Patented in 1986, stereolithography started the rapid prototyping revolution. The technique
builds three-dimensional models from liquid photosensitive polymers that solidify when exposed
to ultraviolet light. As shown in the figure below, the model is built upon a platform situated just
below the surface in a vat of liquid epoxy or acrylate resin. A low-power highly focused UV
laser traces out the first layer, solidifying the model’s cross section while leaving excess areas
Figure 1: Schematic diagram of stereolithography. 7
Next, an elevator incrementally lowers the platform into the liquid polymer. A sweeper re-coats
the solidified layer with liquid, and the laser traces the second layer atop the first. This process is
4. repeated until the prototype is complete. Afterwards, the solid part is removed from the vat and
rinsed clean of excess liquid. Supports are broken off and the model is then placed in an
ultraviolet oven for complete curing.
Stereolithography Apparatus (SLA) machines have been made since 1988 by 3D Systems of
Valencia, CA. To this day, 3D Systems is the industry leader, selling more RP machines than any
other company. Because it was the first technique, stereolithography is regarded as a benchmark
by which other technologies are judged. Early stereolithography prototypes were fairly brittle
and prone to curing-induced warpage and distortion, but recent modifications have largely
corrected these problems.
3.2 Laminated Object Manufacturing
In this technique, developed by Helisys of Torrance, CA, layers of adhesive-coated sheet
material are bonded together to form a prototype. The original material consists of paper
laminated with heat-activated glue and rolled up on spools. As shown in the figure below, a
feeder/collector mechanism advances the sheet over the build platform, where a base has been
constructed from paper and double-sided foam tape. Next, a heated roller applies pressure to
bond the paper to the base. A focused laser cuts the outline of the first layer into the paper and
then cross-hatches the excess area (the negative space in the prototype). Cross-hatching breaks
up the extra material, making it easier to remove during post-processing. During the build, the
excess material provides excellent support for overhangs and thin-walled sections. After the first
layer is cut, the platform lowers out of the way and fresh material is advanced. The platform rises
to slightly below the previous height, the roller bonds the second layer to the first, and the laser
cuts the second layer. This process is repeated as needed to build the part, which will have a
wood-like texture. Because the models are made of paper, they must be sealed and finished with
paint or varnish to prevent moisture damage.
5. Figure 2: Schematic diagram of laminated object manufacturing. 8
Helisys developed several new sheet materials, including plastic, water-repellent paper, and
ceramic and metal powder tapes. The powder tapes produce a "green" part that must be sintered
for maximum strength. As of 2001, Helisys is no longer in business.
3.3 Selective Laser Sintering
Developed by Carl Deckard for his master’s thesis at the University of Texas, selective laser
sintering was patented in 1989. The technique, shown in Figure 3, uses a laser beam to
selectively fuse powdered materials, such as nylon, elastomer, and metal, into a solid object.
Parts are built upon a platform which sits just below the surface in a bin of the heat-fusable
powder. A laser traces the pattern of the first layer, sintering it together. The platform is lowered
by the height of the next layer and powder is reapplied. This process continues until the part is
complete. Excess powder in each layer helps to support the part during the build. SLS machines
are produced by DTM of Austin, TX.
6. Figure 3: Schematic diagram of selective laser sintering.
3.4 Fused Deposition Modeling
In this technique, filaments of heated thermoplastic are extruded from a tip that moves in the x-y
plane. Like a baker decorating a cake, the controlled extrusion head deposits very thin beads of
material onto the build platform to form the first layer. The platform is maintained at a lower
temperature, so that the thermoplastic quickly hardens. After the platform lowers, the extrusion
head deposits a second layer upon the first. Supports are built along the way, fastened to the part
either with a second, weaker material or with a perforated junction.
Stratasys, of Eden Prairie, MN makes a variety of FDM machines ranging from fast concept
modelers to slower, high-precision machines. Materials include ABS (standard and medical
grade), elastomer (96 durometer), polycarbonate, polyphenolsulfone, and investment casting
7. Figure 4: Schematic diagram of fused deposition modeling.
3.4 Solid Ground Curing
Developed by Cubital, solid ground curing (SGC) is somewhat similar to stereolithography
(SLA) in that both use ultraviolet light to selectively harden photosensitive polymers. Unlike
SLA, SGC cures an entire layer at a time. Figure 5 depicts solid ground curing, which is also
known as the solider process. First, photosensitive resin is sprayed on the build platform. Next,
the machine develops a photomask (like a stencil) of the layer to be built. This photomask is
printed on a glass plate above the build platform using an electrostatic process similar to that
found in photocopiers. The mask is then exposed to UV light, which only passes through the
transparent portions of the mask to selectively harden the shape of the current layer.
8. Figure 5: Schematic diagram of solid ground curing. 11
After the layer is cured, the machine vacuums up the excess liquid resin and sprays wax in its
place to support the model during the build. The top surface is milled flat, and then the process
repeats to build the next layer. When the part is complete, it must be de-waxed by immersing it
in a solvent bath. SGC machines are distributed in the U.S. by Cubital America Inc. of Troy, MI.
The machines are quite big and can produce large models.
3.6 3-D Ink-Jet Printing
Ink-Jet Printing refers to an entire class of machines that employ ink-jet technology. The first
was 3D Printing (3DP), developed at MIT and licensed to Soligen Corporation, Extrude Hone,
and others. The ZCorp 3D printer, produced by Z Corporation of Burlington, MA
(www.zcorp.com) is an example of this technology. As shown in Figure 6a, parts are built upon a
platform situated in a bin full of powder material. An ink-jet printing head selectively deposits or
"prints" a binder fluid to fuse the powder together in the desired areas. Unbound powder remains
to support the part. The platform is lowered, more powder added and leveled, and the process
repeated. When finished, the green part is then removed from the unbound powder, and excess
unbound powder is blown off. Finished parts can be infiltrated with wax, CA glue, or other
sealants to improve durability and surface finish. Typical layer thicknesses are on the order of
0.1 mm. This process is very fast, and produces parts with a slightly grainy surface. ZCorp uses
two different materials, a starch based powder (not as strong, but can be burned out, for
investment casting applications) and a ceramic powder. Machines with 4 color printing
capability are available.
9. 3D Systems' (www.3dsystems.com) version of the ink-jet based system is called the Thermo-Jet
or Multi-Jet Printer. It uses a linear array of print heads to rapidly produce thermoplastic models
(Figure 6d). If the part is narrow enough, the print head can deposit an entire layer in one pass.
Otherwise, the head makes several passes.
Sanders Prototype of Wilton, NH (www.solid-scape.com) uses a different ink-jet technique in its
Model Maker line of concept modelers. The machines use two ink-jets (see Figure 6c). One
dispenses low-melt thermoplastic to make the model, while the other prints wax to form
supports. After each layer, a cutting tool mills the top surface to uniform height. This yields
extremely good accuracy, allowing the machines to be used in the jewelry industry.
Ballistic particle manufacturing, depicted in Figure 6b, was developed by BPM Inc., which has
since gone out of business.
Figure 6: Schematic diagrams of ink-jet techniques. 12
4 Applications of Rapid Prototyping
10. Rapid prototyping is widely used in the automotive, aerospace, medical, and consumer products
industries. Although the possible applications are virtually limitless, nearly all fall into one of the
following categories: prototyping, rapid tooling, or rapid manufacturing.
As its name suggests, the primary use of rapid prototyping is to quickly make prototypes for
communication and testing purposes. Prototypes dramatically improve communication because
most people, including engineers, find three-dimensional objects easier to understand than two-
dimensional drawings. Such improved understanding leads to substantial cost and time savings.
As Pratt & Whitney executive Robert P. DeLisle noted: "We’ve seen an estimate on a complex
product drop by $100,000 because people who had to figure out the nature of the object from 50
blueprints could now see it." 13
Effective communication is especially important in this era of
concurrent engineering. By exchanging prototypes early in the design stage, manufacturing can
start tooling up for production while the art division starts planning the packaging, all before the
design is finalized.
Prototypes are also useful for testing a design, to see if it performs as desired or needs
improvement. Engineers have always tested prototypes, but RP expands their capabilities. First,
it is now easy to perform iterative testing: build a prototype, test it, redesign, build and test, etc.
Such an approach would be far too time-consuming using traditional prototyping techniques, but
it is easy using RP.
In addition to being fast, RP models can do a few things metal prototypes cannot. For example,
Porsche used a transparent stereolithography model of the 911 GTI transmission housing to
visually study oil flow. 14
Snecma, a French turbomachinery producer, performed photoelastic
stress analysis on a SLA model of a fan wheel to determine stresses in the blades. 15
4.2 Rapid Tooling
A much-anticipated application of rapid prototyping is rapid tooling, the automatic fabrication of
production quality machine tools. Tooling is one of the slowest and most expensive steps in the
manufacturing process, because of the extremely high quality required. Tools often have
complex geometries, yet must be dimensionally accurate to within a hundredth of a millimeter.
In addition, tools must be hard, wear-resistant, and have very low surface roughness (about 0.5
micrometers root mean square). To meet these requirements, molds and dies are traditionally
made by CNC-machining, electro-discharge machining, or by hand. All are expensive and time
consuming, so manufacturers would like to incorporate rapid prototyping techniques to speed the
process. Peter Hilton, president of Technology Strategy Consulting in Concord, MA, believes
that "tooling costs and development times can be reduced by 75 percent or more" by using rapid
tooling and related technologies. 16
Rapid tooling can be divided into two categories, indirect and
11. 4.2.1 Indirect Tooling
Most rapid tooling today is indirect: RP parts are used as patterns for making molds and dies. RP
models can be indirectly used in a number of manufacturing processes:
Vacuum Casting: In the simplest and oldest rapid tooling technique, a RP positive pattern
is suspended in a vat of liquid silicone or room temperature vulcanizing (RTV) rubber.
When the rubber hardens, it is cut into two halves and the RP pattern is removed. The
resulting rubber mold can be used to cast up to 20 polyurethane replicas of the original
RP pattern. A more useful variant, known as the Keltool powder metal sintering process,
uses the rubber molds to produce metal tools. 17
Developed by 3M and now owned by 3D
Systems, the Keltool process involves filling the rubber molds with powdered tool steel
and epoxy binder. When the binder cures, the "green" metal tool is removed from the
rubber mold and then sintered. At this stage the metal is only 70% dense, so it is
infiltrated with copper to bring it close to its theoretical maximum density. The tools have
fairly good accuracy, but their size is limited to under 25 centimeters.
Sand Casting: A RP model is used as the positive pattern around which the sand mold is
built. LOM models, which resemble the wooden models traditionally used for this
purpose, are often used. If sealed and finished, a LOM pattern can produce about 100
Investment Casting: Some RP prototypes can be used as investment casting patterns. The
pattern must not expand when heated, or it will crack the ceramic shell during
autoclaving. Both Stratasys and Cubital make investment casting wax for their machines.
Paper LOM prototypes may also be used, as they are dimensionally stable with
temperature. The paper shells burn out, leaving some ash to be removed.
To counter thermal expansion in stereolithography parts, 3D Systems introduced
QuickCast, a build style featuring a solid outer skin and mostly hollow inner structure.
The part collapses inward when heated. Likewise, DTM sells Trueform polymer, a
porous substance that expands little with temperature rise, for use in its SLS machines.
Injection molding: CEMCOM Research Associates, Inc. has developed the NCC Tooling
System to make metal/ceramic composite molds for the injection molding of plastics. 18
First, a stereolithography machine is used to make a match-plate positive pattern of the
desired molding. To form the mold, the SLA pattern is plated with nickel, which is then
reinforced with a stiff ceramic material. The two mold halves are separated to remove the
pattern, leaving a matched die set that can produce tens of thousands of injection
4.2.2 Direct Tooling
To directly make hard tooling from CAD data is the Holy Grail of rapid tooling. Realization of
this objective is still several years away, but some strong strides are being made:
12. RapidTool: A DTM process that selectively sinters polymer-coated steel pellets together
to produce a metal mold. The mold is then placed in a furnace where the polymer binder
is burned off and the part is infiltrated with copper (as in the Keltool process). The
resulting mold can produce up to 50,000 injection moldings.
In 1996 Rubbermaid produced 30,000 plastic desk organizers from a SLS-built mold.
This was the first widely sold consumer product to be produced from direct rapid tooling.
Extrude Hone, in Irwin PA, will soon sell a machine, based on MIT’s 3D Printing
process, that produces bronze-infiltrated PM tools and products. 20
Laser-Engineered Net Shaping (LENS) is a process developed at Sandia National
Laboratories and Stanford University that can create metal tools from CAD data. 21
Materials include 316 stainless steel, Inconel 625, H13 tool steel, tungsten, and titanium
carbide cermets. A laser beam melts the top layer of the part in areas where material is to
be added. Powder metal is injected into the molten pool, which then solidifies. Layer
after layer is added until the part is complete. Unlike traditional powder metal processing,
LENS produces fully dense parts, since the metal is melted, not merely sintered. The
resulting parts have exceptional mechanical properties, but the process currently works
only for parts with simple, uniform cross sections. The system has been commercialized
by MTS corporation (www.mts.com)
Direct AIM (ACES Injection Molding): A technique from 3D Systems in which
stereolithography-produced cores are used with traditional metal molds for injection
molding of high and low density polyethylene, polystyrene, polypropylene and ABS
Very good accuracy is achieved for fewer than 200 moldings. Long cycle times
(~ five minutes) are required to allow the molding to cool enough that it will not stick to
the SLA core.
In another variation, cores are made from thin SLA shells filled with epoxy and
aluminum shot. Aluminum’s high conductivity helps the molding cool faster, thus
shortening cycle time. The outer surface can also be plated with metal to improve wear
resistance. Production runs of 1000-5000 moldings are envisioned to make the process
LOMComposite: Helysis and the University of Dayton are working to develop ceramic
composite materials for Laminated Object Manufacturing. LOMComposite parts would
be very strong and durable, and could be used as tooling in a variety of manufacturing
Sand Molding: At least two RP techniques can construct sand molds directly from CAD
data. DTM sells sand-like material that can be sintered into molds. Soligen
(www.3dprinting.com) uses 3DP to produce ceramic molds and cores for investment
casting, (Direct Shell Production Casting).
13. 4.3 Rapid Manufacturing
A natural extension of RP is rapid manufacturing (RM), the automated production of salable
products directly from CAD data. Currently only a few final products are produced by RP
machines, but the number will increase as metals and other materials become more widely
available. RM will never completely replace other manufacturing techniques, especially in large
production runs where mass-production is more economical.
For short production runs, however, RM is much cheaper, since it does not require tooling. RM
is also ideal for producing custom parts tailored to the user’s exact specifications. A University
of Delaware research project uses a digitized 3-D model of a person’s head to construct a
custom-fitted helmet. 23
NASA is experimenting with using RP machines to produce spacesuit
gloves fitted to each astronaut’s hands. 24
From tailored golf club grips to custom dinnerware, the
possibilities are endless.
The other major use of RM is for products that simply cannot be made by subtractive
(machining, grinding) or compressive (forging, etc.) processes. This includes objects with
complex features, internal voids, and layered structures. Specific Surface of Franklin, MA uses
RP to manufacture complicated ceramic filters that have eight times the interior surface area of
older types. The filters remove particles from the gas emissions of coal-fired power plants. 25
Therics, Inc. of NYC is using RP’s layered build style to develop "pills that release measured
drug doses at specified times during the day" and other medical products. 26
5 Future Developments
Rapid prototyping is starting to change the way companies design and build products. On the
horizon, though, are several developments that will help to revolutionize manufacturing as we
One such improvement is increased speed. "Rapid" prototyping machines are still slow by some
standards. By using faster computers, more complex control systems, and improved materials,
RP manufacturers are dramatically reducing build time. For example, Stratasys recently (January
1998) introduced its FDM Quantum machine, which can produce ABS plastic models 2.5-5
times faster than previous FDM machines. 27
Continued reductions in build time will make rapid
manufacturing economical for a wider variety of products.
Another future development is improved accuracy and surface finish. Today’s commercially
available machines are accurate to ~0.08 millimeters in the x-y plane, but less in the z (vertical)
direction. Improvements in laser optics and motor control should increase accuracy in all three
directions. In addition, RP companies are developing new polymers that will be less prone to
curing and temperature-induced warpage.
The introduction of non-polymeric materials, including metals, ceramics, and composites,
represents another much anticipated development. These materials would allow RP users to
14. produce functional parts. Today’s plastic prototypes work well for visualization and fit tests, but
they are often too weak for function testing. More rugged materials would yield prototypes that
could be subjected to actual service conditions. In addition, metal and composite materials will
greatly expand the range of products that can be made by rapid manufacturing.
Many RP companies and research labs are working to develop new materials. For example, the
University of Dayton is working with Helisys to produce ceramic matrix composites by
laminated object manufacturing. 28
An Advanced Research Projects Agency / Office of Naval
Research sponsored project is investigating ways to make ceramics using fused deposition
As mentioned earlier, Sandia/Stanford’s LENS system can create solid metal parts.
These three groups are just a few of the many working on new RP materials.
Another important development is increased size capacity. Currently most RP machines are
limited to objects 0.125 cubic meters or less. Larger parts must be built in sections and joined by
hand. To remedy this situation, several "large prototype" techniques are in the works. The most
fully developed is Topographic Shell Fabrication from Formus in San Jose, CA. In this process, a
temporary mold is built from layers of silica powder (high quality sand) bound together with
paraffin wax. The mold is then used to produce fiberglass, epoxy, foam, or concrete models up to
3.3 m x 2 m x 1.2 m in size. 30
At the University of Utah, Professor Charles Thomas is developing systems to cut intricate
shapes into 1.2 m x 2.4 m sections of foam or paper. 31
Researchers at Penn State’s Applied
Research Lab (ARL) are aiming even higher: to directly build large metal parts such as tank
turrets using robotically guided lasers. Group leader Henry Watson states that product size is
limited only by the size of the robot holding the laser. 32
All the above improvements will help the rapid prototyping industry continue to grow, both
worldwide and at home. The United States currently dominates the field, but Germany, Japan,
and Israel are making inroads. In time RP will spread to less technologically developed countries
as well. With more people and countries in the field, RP’s growth will accelerate further.
One future application is Distance Manufacturing on Demand, a combination of RP and the
Internet that will allow designers to remotely submit designs for immediate manufacture.
Researchers at UC-Berkeley, among others, are developing such a
RP enthusiasts believe that RP will even spread to the home, lending new meaning to
the term "cottage industry." Three-dimensional home printers may seem far-fetched, but the
same could be said for color laser printing just fifteen years ago.
Finally, the rise of rapid prototyping has spurred progress in traditional subtractive methods as
well. Advances in computerized path planning, numeric control, and machine dynamics are
increasing the speed and accuracy of machining. Modern CNC machining centers can have
spindle speeds of up to 100,000 RPM, with correspondingly fast feed rates. 34
Such high material
removal rates translate into short build times. For certain applications, particularly metals,
machining will continue to be a useful manufacturing process. Rapid prototyping will not make
machining obsolete, but rather complement it.